1 Diamond & Related Materials 19 (2010) Contents lists available at ScienceDirect Diamond & Related Materials journal homepage: Fabrication of diamond nanowires for quantum information processing applications Birgit J.M. Hausmann a,b,, Mughees Khan a, Yinan Zhang a, Tom M. Babinec a, Katie Martinick c, Murray McCutcheon a, Phil R. Hemmer d, Marko Lončar a a School of Engineering and Applied Sciences, Harvard University, McKay Lab 219, 9 Oxford Street, Cambridge MA, 02138, United States b Department of Physics, Technische Universität München, James Franck Str., D Garching, Germany c Department of Chemical and Nuclear Engineering, The University of New Mexico, 1 University of New Mexico, Albuquerque, NM , United States d Department of Electrical and Computer Engineering, Texas A&M University, 216H Zachry, TAMU 3128 College Station, Texas , United States article info abstract Article history: Received 28 June 2009 Received in revised form 5 January 2010 Accepted 15 January 2010 Available online 25 January 2010 Keywords: Diamond Nanowire Reactive ion etching ICP Nanostructure We present a design and a top-down fabrication method for realizing diamond nanowires in both bulk single crystal and polycrystalline diamond. Numerical modeling was used to study coupling between a Nitrogen Vacancy (NV) color center and optical modes of a nanowire, and to find an optimal range of nanowire diameters that allows for large collection efficiency of emitted photons. Inductively coupled plasma (ICP) reactive ion etching (RIE) with oxygen is used to fabricate the nanowires. Drop-casted nanoparticles (including Au, SiO 2 and Al 2 O 3 ) as well as electron beam lithography defined spin-on glass and evaporated Au have been used as an etch mask. We found Al 2 O 3 nanoparticles to be the most etch resistant. At the same time FOx e-beam resist (spin-on glass) proved to be a suitable etch mask for fabrication of ordered arrays of diamond nanowires. We were able to obtain nanowires with near-vertical sidewalls in both polycrystalline and single crystal diamond. The heights and diameters of the polycrystalline nanowires presented in this paper are 1 μm and nm, respectively, having a 200 nm/min etch rate. In the case of single crystal diamond (types Ib and IIa) nanowires the height and diameter for different diamonds and masks shown in this paper were μm and nm with etch rates between 190 and 240 nm/min Elsevier B.V. All rights reserved. 1. Introduction Nitrogen-vacancy (NV) color centers embedded in diamond have recently emerged as a promising platform for the realization of robust, room temperature, single-photon sources . The NV center is formed by a two point defect in the diamond lattice: a substitutional nitrogen atom and a vacancy (missing carbon atom) trapped at an adjacent lattice position. It can exist in two charged states NV 0 and NV out of which the NV center is suitable for quantum operations due to the electron's spin kinetics. The luminescence spectrum of an NV color center consists of a broad (640 nm to 780 nm) phonon side-band (PSB) and a zero-phonon line (ZPL) at 637 nm [2,3]. NV centers combine the key advantages of isolated atomic systems with solidstate integration, and have the following unique optical properties: (i) room temperature operation, (ii) little inhomogeneous broadening, and (iii) deterministic positioning using ion implantation. Moreover, the NV center stands out among solid-state systems because its electronic spin can be prepared, manipulated, and measured with optical and microwave excitations . Corresponding author. School of Engineering and Applied Sciences, Harvard University, McKay Lab 219, 9 Oxford Street, Cambridge MA, 02138, United States. Tel.: address: (B.J.M. Hausmann). However, NV centers also interact with their environment leading to decoherence in the presence of nearby nitrogen spins. Hence it is important to enhance the NV center emission yield (photon production rate) as well as increase the collection efficiency of emitted photons. This can be achieved by embedding NV centers within optical structures including cavities, microdisks, waveguides and nanowires. NV optical transition is in the visible (637 nm), which limits the choice of materials that can be used to realize optical structures. Diamond itself is a suitable platform having a reasonably high refractive index (n=2.43). Baldwin et al.  have fabricated 2D photonic crystal (PhC) slabs in polycrystalline diamond (poly-d) on insulator (DOI) films. Similarly, Wang et al. [6,7] have demonstrated the fabrication of optical microdisk resonators and 2D PhC in polycrystalline diamond films using E-Beam Lithography (EBL) and Reactive Ion Etching (RIE). The characterization of poly-d microdisks and photonic crystal cavities has shown scattering losses due to the polycrystalline nature of the diamond film. Moreover, the emission from polycrystalline diamond itself can obscure single-photon emission from an embedded NV center. Hence, defect-free single crystal diamond (sc-d) films are needed for quantum information processing (QIP) applications. High-quality sc-d films can only be homo-epitaxially grown on the diamond substrate and therefore the needed index contrast for the realization of nanophotonic devices does not exist. Olivero et al.  have used ion-beam implantation followed by sacrificial removal of /$ see front matter 2010 Elsevier B.V. All rights reserved. doi: /j.diamond
2 622 B.J.M. Hausmann et al. / Diamond & Related Materials 19 (2010) implanted graphitized (damaged) layer to fabricate thin sc-d films. Based on this approach fabrication of sc-d waveguides  and microdisk resonators  has been demonstrated. However, the ion implantation may create additional NV centers and may render such thin films unsuitable for QIP applications. Optical structures fabricated in a GaP layer bonded on top of a diamond film  have also been reported. Approaches based on diamond nanocrystals containing NV centers embedded within a silicon-nitride photonic crystal structure has been examined theoretically . Other works include positioning diamond nanocrystals on top of wide bandgap materials such as GaP  and silicon-dioxide  as well as metallic nanostructures . In this work an alternative approach has been explored based on the fabrication of nanowires in diamond containing NV centers. Recently, Friedler et al.  have theoretically demonstrated a 90% extraction efficiency of emitted photons from single-photon sources like quantum dots embedded within semiconductor nanowires. We first examine an optimal nanowire diameter that maximizes the overall collection efficiency of photons emitted from an NV center. Next, we developed a fabrication procedure for the creation of diamond nanowires directly in high-quality sc-d substrates utilizing RIE and as needed EBL. Our procedure uses oxygen as a reactive gas in an inductively coupled plasma (ICP) RIE. In the past a two step procedure for diamond nanorods based on hydrogen treated sc-d whiskers has been pursued . Other fabricated structures in poly- and sc-d based on reactive ion etching (RIE) include microlenses [18,19], porous diamond , field emitters , waveguides , atomic force microscopy (AFM) tips , disks ,cones and cylinders,nanopillars, microcylinders  and resonator arrays for RF signal processing . As masks, we investigated two main approaches: (i) nanoparticles deposited using drop-casting (Au, SiO 2,Al 2 O 3 ), and (ii) masks defined by EBL using positive as well as negative resist. We also investigated two types of substrates: (i) poly-d films on insulator, and (ii) sc-d diamonds grown via high-pressure high-temperature (HPHT) and chemical vapor deposition (CVD) processes. 2. Design and modeling First, we studied the emission from an NV center (modeled as a dipole) in a diamond nanowire using FDTD simulations. We assume a circular cross section of the nanowire with a diameter d, and consider the two general polarization scenarios for a dipole/nanowire system: dipole polarization perpendicular (s-polarized) and parallel (p-polarized) to the nanowire axis. The dipole associated with an NV center in (100) diamond can be represented using combination of these two dipoles, since it is polarized in the (111) plane. At different wavelengths within the NV center's radiation spectrum (637 nm 780 nm), the number of collected photons per second can be expressed as Γ(λ) η(λ) where Γ is the emission rate (reciprocal to the lifetime) and η the collection efficiency. The collection efficiency can be dramatically improved in diamond nanowires compared with bulk diamond, as demonstrated in Fig. 1. Thesefield profiles show that the major portion of light emitted from an NV center in bulk diamond leaks to the substrate due to significant total internal reflection at the diamond air interface, whereas in a diamond nanowire the fundamental HE 11 mode is the dominant emission channel for a dipole polarized perpendicular to the nanowire axis (in the xy plane) (inset) .Thiswaveguidemode directs the light propagating in the nanowire, and is scattered vertically as it exits from the top nanowire facet. This process allows for efficient collection using an objective lens positioned above . InFig. 2a we show the coupling efficiency, α, between the NV center and the nanowire waveguide mode as a function of the nanowire diameter, for wavelength λ=637 nm. It can be seen that, in the case of s-polarized dipole, more than 80% of emitted photons can couple to the nanowire mode for a broad range of nanowire diameters (180 nm 230 nm). We choose to work with 200 nm diameter nanowires in order to optimize the coupling efficiency. Photon collection efficiencies can be quantified from the far-field profile of power emitted upward, shown in Fig. 2band c. An objective lens with a numerical aperture NA=0.95, positioned above the nanowire, can collect light emitted into the solid angle of 72 (represented by shaded areas in the far-field emission profiles). It can be seen that in the case of both s- and p-polarized dipoles, almost 100% of photons emitted from the nanowire can be collected with the lens. It is interesting to note that this is true even for p-polarized dipole despite the fact that it cannot couple to the nanowire waveguide mode due to the symmetry mismatch. In this case, however, large collection efficiency is enabled by coupling to radiative modes that are also modified by the presence of the nanowire. Finally, comparing a dipole in a nanowire (red line in Fig. 2b and c) with a dipole in a bulk diamond crystal (blue line), we find that the nanowire geometry provides one and two orders of magnitude improvement in the collection efficiency in the case of s-polarized and p-polarized dipole, respectively. We also evaluated the total emission rate (the reciprocal of lifetime) of an NV center in a nanowire, and found that it is dependent on the NV center's position: Fabry Perot resonances, formed due to the (weak) reflection of a waveguide mode from the nanowire's facets, can modify the emission rate of s-polarized dipole. We introduce the enhancement factor EðλÞ = Γλ ð Þ Γ 0 ðλþ where Γ 0 is the emission rate of the quantum emitter Fig. 1. Field profile of the E-field's radial component (E r ) in the case of a 2 μm long, 200 nm diameter diamond nanowire (left) and a bulk diamond (right). The dipole is polarized parallel to the interface, emitting at λ =637 nm (zero-phonon line wavelength of NV center). The fundamental nanowire waveguide mode (HE 11 ) (inset) is the dominant decay channel for the nanowire case.
3 B.J.M. Hausmann et al. / Diamond & Related Materials 19 (2010) Fig. 2. (a) Coupling efficiency α as a function of the nanowire diameter at λ=637 nm. The dipole is assumed to be placed at the center of the nanowire with a polarization perpendicular to the nanowire axis (s-polarized). b and c: the far-field profile of power emitted from a (b) s-polarized and (c) p-polarized (parallel to the nanowire axis) dipole embedded at the center of a nanowire with d=200 nm. Blue lines, in both b and c, show far-field profiles of emitter embedded in the bulk diamond crystal. The shaded areas denote the light that can be collected using an objective lens with an NA of Calculated values of collection efficiency η for nanowire and bulk, for both polarizations, are also indicated. in a homogeneous diamond medium. For λ=637 nm and d=200 nm, the enhancement factor is in the range of , depending on the dipole position along the nanowire positions. It is interesting to note that the collection efficiency for s-polarized dipole is maximized (Fig. 2b) when destructive interference occurs between downward emitted photons and photons reflected from the top nanowire facet (Fig. 1). This case favors upward emission at the expense of slightly increased radiative lifetime. In order to estimate the total number of photons that can be collected from a nanowire geometry, it is important to take into account both s- and p-polarized components of NV dipole, as well as its broad-band emission due to the phonon side-band. The total number of collected photons is obtained by averaging over wavelengths and polarizations, by using following (unitless) figure of merit Z = E ð λ; σ Þηλ; ð σþγ 0ðλÞdσdλ 2π Γ 0 ðλþdλ where σ denotes the polarization angle. Using this figure of merit, we find that the nanowire geometry provides an order of magnitude improvement (Z 30%) over the bulk diamond case (Z 3.3%). 3. Materials and methods We used two types of diamond samples based on their crystalline nature: (a) poly-d films and (b) types Ib and IIa sc-ds synthesized via HPHT and CVD processes respectively. While sc-ds are needed to realize single-photon sources, poly-d films have been used to optimize the etch recipe due to their low-cost and availability in large quantities. The poly-d samples were diamond on insulator (DOI) AQUA 25 wafers (2 μm poly-d film on 1 μm thermal SiO 2 on a Si substrate) from Advanced Diamond Technologies, Inc. The sample size was about 3 5mm 3 5 mm. Prior to mask deposition and reactive ion etching all poly-d samples were solvent cleaned. The nitrogen rich HPHT Ib and very pure (nitrogen content < 0.1 ppm) CVD IIa sc-ds were obtained from Element6 (E6), and were 3 mm 3 mm in size. We also used a CVD sc-d from Apollo Diamond, Inc. All sc-d samples had a <100> crystal orientation and prior to mask deposition, and etching all sc-ds were cleaned for about 45 min in a boiling 1:1:1 (Nitric:Perchloric: Sulfuric) acid bath. This aggressive etch was not used with the poly-d samples as it was damaging the DOI film. Three major types of etch masks have been explored in this work, each of which required a slightly different fabrication approach. The adopted fabrication processes are shown in Fig. 3. The etch masks were prepared as discussed below. (A) Nanoparticle mask, deposited via drop-casting: in this approach drop-casted nanoparticles have been used as an etch mask. Au colloids suspended in DI water were obtained from Ted Pella, Inc. The nominal particle sizes were 100 nm and 250 nm. However, our measurements indicated a large variation with mean particle diameters of 140 nm and 350 nm respectively. The concentrations were particles/ml and particles/ml for the 100 nm and 250 nm colloids respectively. Au nanoparticles were further diluted in 1:1 and 1:2 ratio with DI water before dispersing on the samples. A suspension of SiO 2 nanoparticles (Corpuscular, Inc.) with a diameter of 213 nm and a 5% particle concentration in a 10 ml solution was also used. The SiO 2 particle-size variation was smaller than 8%. Finally, Al 2 O 3 powder from Alfa Aesar, Inc. with 200 nm and nm diameters were used. (B) Au mask defined via a lift-off process: in this approach, evaporated Au was used as an etch mask as illustrated in Fig. 3. Bilayer PMMA from MicroChem Corp was used to define an etch pattern using a 100 kv Elionix e-beam tool. Dosages were varied from 800 μc/cm 2 to 1600 μc/cm 2. Next, 10 nm Cr and 200-nm Au evaporation followed by a lift-off process was used to define a metal etch mask. (C) Spin-on-glass (HSQ) mask defined by EBL: flowable oxide (FOx 17) from Dow Corning was diluted with MIBK in 1:2 and 1:1 ratios. Dosages from 4800 μc/cm 2 to 8000 μc/cm 2 were used to expose FOx resist. An ICP RIE system (UNAXIS shuttleline) was used to transfer the mask pattern into all the diamond samples. An etch recipe having 30 sccm oxygen flow rate, 100 W Bias power, 700 W ICP power at a 10 mtorr chamber pressure was used and will be discussed in the next section. After RIE, gold (type TFA, Transene) and chrome etchant (type 1020, Transene) were used in approaches (A) and (B) to remove the remaining Au/Cr mask. In case (C), an HF (49%, aq) wet etch was performed to remove the remaining FOx mask. All images were taken with a Zeiss SUPRA field emission scanning electron microscope (FESEM) under a 86 tilt unless noted otherwise. The secondary electron (SE) detector and an acceleration voltage of 5 kv was used.
4 624 B.J.M. Hausmann et al. / Diamond & Related Materials 19 (2010) Fig. 3. Fabrication process schematic. (a) Drop casting of nanoparticles (Al 2 O 3, Au, SiO 2 ) followed by etching. (b) EBL-defined Au evaporation and etching. (c) EBL-defined FOx mask (flowable oxide, a spin-on-glass resist) and etching. 4. Results and discussion 4.1. Etch recipe variation Based on our design presented earlier, an etch recipe and etch mask that yield wires with vertical profile and high selectivity are needed. Several dry etch parameters were varied in order to obtain an acceptable wire profile. The results are presented in Fig. 4 and the etch parameter variations, heights and diameters are summarized in Table 1. Waist diameter refers to the thickest part of the nanowire and the taper angle is calculated based on the waist and the bottom diameter. The tabulated variations are for a 5 min etch using Au colloids with a diameter of 250 nm as an etch mask on poly-d samples. A height of 1 μm was determined in most cases, except for (d) and (g) the height was 1.1 μm and 0.7 μm respectively. Recipe (a) resulted in unwanted grass. Raising the temperature and decreasing the pressure resulted in smooth bottom surfaces (no grass) but introduced a noticeable mask erosion at the top (b). Further increase in temperature resulted in re-appearance of the grass (c) and a reduced etch depth. Slightly undercut wires are obtained with a higher oxygen flow rate of 45 sccm (recipe d) and a reduced temperature compared to recipe (b) as shown in Fig. 4d. The increased flow rate and reduced temperature also increased the mask erosion at the top of the nanowires. To consider the effect of an increased ion density the ICP power was increased by 30% (recipe (e)) while reducing the oxygen flow rate compared to recipe (d) by 33%. This yielded in a 3.5 times larger undercut compared to recipe (d). In recipe (f) (Fig. 4f) the chamber pressure was decreased to 3 mtorr, the bias power was increased to 200 W and the oxygen flow rate was reduced to 30 sccm compared to recipe (d) which leads to mask erosion and excessive etching. In Fig. 4g the etch recipe with 20 mtorr and 200 W was tested to minimize mask erosion by increasing the pressure compared to recipe (f). This resulted in relatively little mask erosion, an over cut wire profile and a reduced etch depth. To minimize the mask erosion observed in recipe (b) and (d) (Fig. 4b, d), the oxygen flow rate was reducedto30sccmcomparedtorecipe(d)astabulatedinrecipe(h). This gave a near-vertical wire profile with minimal mask erosion as shown in Fig. 4h and was used as the basic recipe for etching all the diamond samples presented in this paper Comparison of nanoparticle etch mask In order to improve the etch selectivity, different nanoparticle masks were also evaluated. A close up view of poly-d wires obtained using the optimized etch recipe with different nanoparticle masks are shown in Fig. 5. The Al 2 O 3 mask was tried first. A similar mask has been used successfully to build micropost-cavities with embedded quantum dots in the past . Al 2 O 3 nanoparticles were deposited from both suspension and powder form. In the latter case, the samples were dipped top-down into the powder. Al 2 O 3 was found to be an ideal etch mask with no appreciable erosion. A 4 min oxygen etch gave a height of the etched diamond structure of 1 μm and a diameter of 200 nm both at the top and the bottom, as shown in Fig. 5a. The thickest diameter was 230 nm. The particle height was 210 nm and its thickest diameter was 230 nm. However, Al 2 O 3 nanoparticles were found to be clumping together, resulting in large etched features with random cross-sectional profiles (Fig. 5a), which was not desirable. Better uniformity and isolation of individual Al 2 O 3 nanoparticles can be achieved by modifying the Al 2 O 3 nanoparticles deposition process.
5 B.J.M. Hausmann et al. / Diamond & Related Materials 19 (2010) Fig. 4. Summary of etch recipe variations in DOI after a 5 min oxygen dry etch, using 250 nm Au particles as mask. Labels a through h correspond to etch recipes with the same name in Table 1.
6 626 B.J.M. Hausmann et al. / Diamond & Related Materials 19 (2010) Table 1 Summary of all etch variations. Straight wires were obtained with the optimized etch recipe (last row) for poly-d. Rec. Temp. Press. Bias ICP O 2 Etch rate Bottom Top Waist Taper angle Result C mtorr W W sccm nm/min nm nm nm (a) RT Grass (b) Undercut (c) Grass (d) RT Straight (e) RT Undercut (f) RT Erosion (g) RT Over cut (h) RT Straight Due to better size and shape uniformity SiO 2 nanoparticles were also evaluated. Fig. 5b shows the etch results obtained using individual SiO 2 nanoparticles. Poor selectivity and a high mask erosion were observed, since SiO 2 particles were etched at a rate of 40 nm/min. The mask erosion also resulted in a tapered nanowire profile. The height of the wires after a 5 min oxygen etch was 1 μm, and the diameter varies from 342 nm on the bottom to 20 nm at the top. The SiO 2 particles did not survive the etch. Fig. 5c shows a 900 nm high nanowire obtained with 250 nm gold particles as the mask. The diameter varied from 275 nm on the bottom to a maximum of 310 nm and 250 nm at the top. The particle shown in this image measures 245 nm in diameter and 130 nm in height. The etch time was 5 min. The Au nanoparticles were the easiest to disperse, resulting in single nanoparticles requiring no further processing steps. Using 250 nm nanoparticles, a 5 min etch resulted in 1 μm tall nanowires, as shown in Fig. 6a. The diameter varied from 260 nm at the bottom and top to 280 nm as thickest diameter. The etch rates of the mask and the DOI film were determined to be 25 nm/min and 200 nm/min, respectively. This results in an etch selectivity of 8:1. The wires created in poly-d have a near-vertical profile. Fig. 6a and b show a comparison of poly-d wires etched using 250 nm and 100 nm nanoparticles. The use of 100 nm Au particles (1:200 dilution) resulted in similar etch rates but with a tapered nanowire profile, which can be attributed to significant mask erosion in the case of the small gold nanoparticles (Fig. 6b). However, such tapered profile may be beneficial for achieving high extraction efficiency for photons emitted from NV centers embedded within nanowires [16, 29]. The height was 0.9 μm and the thickest diameter is about 120 nm Single crystal diamond nanowires Due to the ease in dispersing and the reasonable etch selectivity of 8:1, Au nanoparticles were drop-casted on E6 CVD IIa and E6 HPHT Ib samples. The samples were etched for 5 min and 10 min, respectively, the results of which are shown in Fig. 7. After a 5 min etch, the nanowires are broadened in the bottom half and are almost straight in the upper half, as indicated in Fig. 7a. The top bottom wire height is 1.1 μm. The diameters vary from 350 nm at the bottom of the wires to 230 nm at the top just beneath the remaining particles. The etching time was 5 min. An etch rate of 220 nm/min was measured. Ib sc-d nanowires after a 10 min etch are shown in Fig. 7b. The gold particle mask was almost completely eroded after this time and thus the upper part of the nanowire comes out tapered. The etch rate is 190 nm/min. The top bottom height is 1.9 μm and the diameters vary from 470 nm at the bottom of the wires to 190 nm at the top beneath the remaining particles. The mask etch rate was in both cases nm/min. Thus the etch selectivity was found to be 8:1 and 9:1 for Ib and IIa sc-ds respectively. While the nanoparticle drop-casting approach provides a simple method to realize a large number of randomly positioned diamond nanowires, ordered arrays of nanowires are desirable for the characterization of functional devices. Another factor to consider is the effect of the near-spherical shape of the nanoparticle etch mask on Fig. 5. Poly-D nanowires obtained with (a) Al 2 O 3 powder ( 200 nm in diameter), (b) SiO 2 particles (210 nm in diameter) and (c) 250 nm gold particles as mask, etched with the oxygen recipe. (a) The height is 1 μm and the diameter is 200 nm both on the top and the bottom. The thickest diameter is 230 nm. The particle height is 210 nm and its thickest diameter is 230 nm. (b) The height of the wires is 1 μm and the diameter varies from 342 nm on the bottom to 20 nm at the top. (c) The nanowire is 900 nm high. The diameter varied from 275 nm on the bottom, to a maximum of 310 nm and 250 nm at the top. The particle measures 245 nm in diameter and 130 nm in height. The etch time was 5 min.
7 B.J.M. Hausmann et al. / Diamond & Related Materials 19 (2010) Fig. 6. Poly-D nanowires after a 5 min oxygen etch. (a) 250-nm Au colloids served as etch mask. The top bottom height of the wires is 1 μm and the thickest diameter is about 280 nm. The diameter at the bottom of the wires is 260 nm. Inset: close-up view of some wires. Figure b shows poly-d nanowires obtained with a 1:200 dilution of 100-nm Au colloids as a mask. The top bottom height of the wires is 0.9 μm and the thickest diameter is about 120 nm. the etch profile of nanowires. Due to these reasons, EBL-defined masks have also been considered in this work. Ordered arrays of varying diameters between 100 nm and 250 nm, which cover the range of the optimum diameters as presented in Section 2, were patterned on sc-d samples. Wire-to-wire distances (periodicity) of 2 μm and 3 μm were used. The distance was chosen to allow ease in characterization of individual nanowires using a custom built confocal micro-photoluminescence setup without introducing any stray signal from neighboring nanowires. Details of the experimental setup and results will be presented in a future publication. EBL using PMMA resists followed by a lift-off process was used to realize an evaporated Cr/Au metal mask, as described in Section 3 (Fig. 3). The results of etching E6 IIa CVD diamond with such a mask are shown in Fig. 8. A 10 min oxygen etch produces 2.2 μm high nanowires. The diameter at the top of the wires of this array is 160 nm and at the bottom 490 nm. The diamond etch rate is 220 nm/min, whereas the etch rate of the evaporated gold is 26 nm/ min. In the inset a wire is shown with the remaining mask after a 5 min etch. The mask is 120 nm high and the diameter of the wire is 200 nm at the top. Again, an over cut etch profile is observed in the case of sc-d nanowires. As mentioned above, the same recipe resulted in a vertical nanowire profile in the case of poly-d nanowires. We expect that an increase in the isotropic etch component of our recipe would result in straighter nanowires. Au nanoparticles and evaporated Au gave a similar etch rate of 25 nm/min. In order to further simplify the fabrication procedure, we used FOx (which is a negative e-beam resist) as an etch mask, as mentioned in Section 3 (Fig. 3). This required no metal evaporation and lift-off. The profile of the wires in E6 Ib sc-d can be seen in Fig. 9. Fig. 7. Sc-D nanowires obtained with 250 nm Au colloids as a mask for oxygen etching. (a) E6 IIa sc-d nanowires with a top bottom wire height of 1.1 μm. The diameters vary from 350 nm at the bottom of the wires to 230 nm at the top. The etching time was 5 min. Inset: close-up view of one wire. (b) E6 Ib nanowires with a top bottom height of 1.9 μm. The diameters vary from 470 nm at the bottom of the wires to 190 nm at the top beneath the remaining particles. The etching time was 10 min. Inset: magnified view of three wires. Fig. 9a shows 2.3 μm high wires. The EBL-written diameter of this array was 150 nm. The measured diameters at the broadest part of the top and the bottom are 110 nm and 310 nm, respectively. At the thinnest part of the wires the diameter is 70 nm. In Fig. 9c, an array of 2.2 μm high nanowires with a bottom diameter of 226 nm are shown (written diameter: 100 nm). We found the etch rate of FOx to Fig. 8. Sc-D nanowires obtained in a IIa CVD diamond. After a 10 min oxygen etch using an EBL-defined evaporated Cr/Au (10/200) nm mask. The height is 2.2 μm from top to bottom, the remaining mask on this set of wires is 60 nm high. The diameter just beneath the mask is 160 nm and at the bottom 490 nm. Inset: the etch time was 5 min, the remaining mask on this set of wires is 120 nm high. The diameter just beneath the mask is 200 nm.
8 628 B.J.M. Hausmann et al. / Diamond & Related Materials 19 (2010) be smaller than 10 nm/min, which is almost three times better than the metal mask. In order to improve the etch profile of sc-d nanowires and obtain nanowires with vertical sidewalls, we changed our etch recipe slightly by varying the ICP power. Based on the profile we obtained with our base etch recipe, we decided to decrease the chemical etch rate after a few minutes and then increase it to prevent the broadening of the wires (Figs. 8 and 9). We used our usual recipe for 2 min, decreased the ICP power to 600 W for 3 min and then ramped up to 1000 W for 5 min. The results can be seen in Fig. 10a. The periodicity and diameter of the wires used in EBL are 3 μm and 200 nm respectively. We were able to realize 1.9 μm tall nanowires with near-vertical profile (bottom diameter of 260 nm) and a tapered top due to the high ICP power causing mask erosion. This can be minimized by using a thicker FOx mask film. As mentioned earlier, however, a tapered profile may be preferable  for increasing the extraction collection efficiency from emitters embedded inside nanowires. Based on the above recipe optimization results, an ultra pure type IIa diamond from Apollo Diamond, Inc. was also etched with slightly different etch step lengths: 1.5 min, 3 min and 5.5 min. The profile of the 2.4um tall wires with a periodicity of 3 μm can be seen in Fig. 10b and c. Nanowires with a bottom diameter of 340 nm are shown in Fig. 10b (EBL-written diameter: 220 nm). The thinnest and top diameters are 190 nm and 210 μm respectively. Another array with diameters ranging from 170 nm at the bottom to 60 nm at the nanowire waist and 120 nm at the top can be seen in Fig. 10c. The diameter used in EBL was 140 nm. The wire etch rate was measured as 240 nm/min. 5. Conclusion Fig. 9. Sc-D wires formed in a Ib HPHT diamond. FOx was used to produce an array of pillar-shaped mask with EBL. The mask was then transferred to the substrate during a 10 min oxygen etch and subsequently removed. (a) One pattern of wires with the same diameters. (b) The height of the wires is 2.3 μm from top to bottom. The diameters at the broadest part of the top and the bottom are 110 nm and 310 nm respectively. At the thinnest part of the wires the diameter is 70 nm. Inset: one wire with the remaining FOx mask after etching (different diameter). (c) One array of 2.2 μm high nanowires with a bottom diameter of 226 nm. In this work, we have presented the design and fabrication of diamond nanowires. Our modeling shows an optimal range of diameters for coupling (>80%) the Nitrogen Vacancy (NV) center emission to the propagating waveguide mode inside the diamond nanowire, and collecting that emission with a high extraction efficiency using a 0.95 NA objective. We have also investigated diamond etching of poly-d and sc-d nanowires. We have summarized the etch rates of all diamond types in Table 2. Nanowires with nearvertical profiles were fabricated using an oxygen ICP RIE recipe. Al 2 O 3, Au and SiO 2 particles, evaporated Au and FOx e-beam resist were evaluated as an etch mask. It was found that Al 2 O 3 nanoparticles were Fig. 10. (a) Sc-D (Ib HPHT) wires after a 10 min oxygen etch. The FOx mask was removed. The height of the wires is 1.9 μm from top to bottom and the diameter at the bottom is 260 nm. (b and c) Sc-D nanowires formed in a diamond from Apollo Diamond after removing the FOx mask. Their height is 2.4 μm and the distance between each nanowire is 3 μm. (b) Nanowires with a bottom diameter of 340 nm. The thinnest and top diameters are 190 nm and 210 nm respectively. (c) The diameter varies from 170 nm at the bottom, to 60 nm at the nanowire waist and 120 nm at the top.
9 B.J.M. Hausmann et al. / Diamond & Related Materials 19 (2010) Table 2 Summary of the etch rates in the different diamond types. For the Apollo IIa a different etch recipe has been used (see Section 4.3), for the other diamond types we used the etch recipe introduced in Section 3. Type Etch rate Etch time nm/min min Poly-D Ib sc-d IIa sc-d (E6) IIa sc-d (Apollo Diamond) most resistant to etching. Au nanoparticles and evaporated Au gave a similar etch rate, while FOx e-beam resist gave an etch rate of 10 nm/ min and was found to be the most suitable mask based on our fabrication process. The crystalline nature of the samples affected the etch profile and required different etch parameters to obtain nearly vertical etch profiles of the nanowires. Polycrystalline and type Ib single crystal diamond were found to etch at ( ) nm/min, whereas type IIa single crystal diamonds were found to etch at about ( ) nm/min. We believe that our nanowire work and the diamond nanophotonic technology that we are developing will play an important role as an enabling platform for fundamental quantum information processing applications, as well as bio-sensing applications based on magnetometry . Acknowledgments This work is supported in part by the DARPA Quest program (PM Jagdeep Shah), NSF NIRT grant, and Harvard NSEC. The authors wish to acknowledge the help during the search for a suitable nanowire fabrication process by Chih-Hsun Hsu and Jeffrey Shainline (Jimmy Xu's lab at Brown University). The authors thank Advanced Diamond Technologies and Apollo Diamond for providing diamond test samples. Fruitful discussions with Philippe Lalanne and help from Maja Cassidy and Ben Hatton are acknowledged. One of the authors (B. H.) wishes to cordially thank Anna Fontcuberta i Morral and Jonathan Finley for their support. Most of the fabrication work was performed at the Center for Nanoscale Sciences (CNS) Nanofabrication facility at Harvard University, a member of the National Nanotechnology Infrastructure Network (NNIN), which is supported by the National Science Foundation under NSF award no. ECS Disclaimer: The views, opinions, and/or findings contained in this publication are those of the authors and should not be interpreted as representing the official views or policies, either expressed or implied, of the Defense Advanced Research Projects Agency or the Department of Defense. References  C. Kurtsiefer, S. Mayer, P. Zarda, H. Weinfurtner, Phys. Rev. Lett. 85 (2000) 290.  N. Reddy, N. Manson, E. Krausz, J. Lumin. 38 (1987) 46.  F. Jelezko, C. Tietz, A. Gruber, I. Popa, A. Nizovtsev, S. Kilin, J. Wrachtrup, Single Mol. 2 (2001) 255.  T. Gaebel, M.L. Domhan, I. Popa, C. Wittmann, P. Neumann, F. Jelezko, J.R. Rabeau, N. Stavrias, A.D. Greentree, S. Prawer, J. Meijer, J. Twamley, P.R. Hemmer, J. Wrachtrup, Nat. Phys. 2 (2006) 408.  J.W. Baldwin, M.K. Zalalutdinov, T. Feygelson, J.E. Butler, B.H. Houston, J. Vac. Sci. Technol. B 24 (2006) 50.  C.F. Wang, Y.-S. Choi, J.C. Lee, E.L. Hu, J. Yang, J.E. Butler, Appl. Phys. Lett. 90 (2007)  C.F. Wang, R. Hanson, D.D. Awschalom, E.L. Hu, T. Feygelson, J. Yang, J.E. Butler, Appl. Phys. Lett 91 (2007) 201,112.  P. Olivero, S. Rubanov, P. Reichart, B. C. Gibson, S. T. Huntington, J. Rabeau, A. D. Greentree, J. Salzman, D. Moore, D. N. Jamieson, and S. Prawer, Ion-beam-assisted lift-off technique for three-dimensional micromachining of freestanding singlecrystal diamond, Adv. Mater., 17.  M.P. Hiscocks, K. Ganesan, B.C. Gibson, S.T. Huntington, F. Ladouceur, S. Prawer, Opt. Express 16 (24) (2009) 19,512.  C.F. Wang, and E.L. Hu, Fabrication of suspended single crystal diamond devices by electrochemical etch, J. Vac. Sci. Technol. B, 25 (3), (2007) (2005).  K.-M.C. Fu, P.E. Barclay, I. Aharonovich, S. Prawer, A.M. Holm, R.G. Beausoleil, Appl. Phys. Lett. 93 (2008) 234,107.  M.W. McCutcheon, M. Lončar, Opt. Express 16 (2008) 19,136.  K. Rivoire, A. Faraon, J. Vučković, Appl. Phys. Lett. 93 (2008)  P.E. Barclay, O. Painter, C. Santori, K.-M. Fu, R.G. Beausoleil, Coherent interference effects in a nano-assembled optical cavity-qed system, ArXiv: ,  S. Schietinger, M. Barth, T. Aichele, O. Benson, Nano Lett. 9 (4) (2009)  I. Friedler, C. Sauvan, J.P. Hugonin, P. Lalanne, J. Claudon, J.M. Gérard, Opt. Express 17 (2009)  Y. Ando, Y. Nishibayashi, A. Sawabe, Diam. Relat. Mater. 14 (2004) 633.  C.L. Lee, E. Gu, M.D. Dawson, I. Friel, G.A. Scarsbrook, Diam. and Relat. Mater. 17 (2008)  E. Gu, H.W. Choi, C. Liu, C. Griffin, J.M. Girkin, I.M. Watson, M.D. Dawson, G. McConnell, A.M. Gurney, Appl. Phys. Lett. 84 (15) (2004)  H. Shiomi, Jpn. J. Appl. Phys. 36 (1997)  T. Yamada, P.R. Vinod, D.-S. Hwanga, H. Yoshikawa, S. Shikata, N. Fujimori, Diam. and Relat. Mater. 14 (2005)  T. Yamada, H. Yoshikawa, H. Uetsuka, S. Kumaragurubaran, N. Tokuda, S. Shikata, Diam. Relat. Mater. 16 (2007) 996.  D. Hwang, T. Saito, N. Fujimori, Diam. and Relat. Mater. 13 (2004)  M. Larsson, K.N. Dinyari, H. Wang, Nano Lett. 9 (4) (2009)  Y. Ando, Y. Nishibayashi, K. Kobashi, T. Hirao, K. Oura, Diam. Relat. Mater. 11 (2002) 824.  J.W. Baldwin, M.K. Zalalutdinov, T. Feygelson, B.B. Pate, J.E. Butler, B.H. Houston, Diam. Relat. Mater. 15 (2006)  A.V. Maslov, C.Z. Ning, Opt. Lett. 26 (6) (2004) 572.  J. Vučković, D. Fattal, C. Santori, G.S. Solomon, Y. Yamamoto, Appl. Phys. Lett. 82 (21) (2003).  N. Gregersen, T.R. Nielsen, J. Claudon, J.-M. Gérard, J. Mørk, Opt. Lett. 33 (15) (2008)  J.R. Maze, P.L. Stanwix, J.S. Hodges, S. Hong, J.M. Taylor, P. Cappellaro, L. Jiang, M.V. Gurudev Dutt, E. Togan, A.S. Zibrov, A. Yacoby, R.L. Walsworth, M.D. Lukin, Nat. 455 (2008) 644.
III. Wet and Dry Etching Method Environment and Equipment Advantage Disadvantage Directionality Wet Chemical Solutions Atmosphere, Bath 1) Low cost, easy to implement 2) High etching rate 3) Good selectivity
OSE6650 - Optical Properties of Nanostructured Materials Optical Properties of Nanostructured Materials Fall 2013 Class 3 slide 1 Challenge: excite and detect the near field Thus far: Nanostructured materials
Scanning Near Field Optical Microscopy: Principle, Instrumentation and Applications Saulius Marcinkevičius Optics, ICT, KTH 1 Outline Optical near field. Principle of scanning near field optical microscope
email@example.com Nanometer-scale imaging and metrology, nano-fabrication with the Orion Helium Ion Microscope Bin Ming, András E. Vladár and Michael T. Postek National Institute of Standards and Technology
CMOS Processing Technology Silicon: a semiconductor with resistance between that of conductor and an insulator. Conductivity of silicon can be changed several orders of magnitude by introducing impurity
Demonstration of sub-4 nm nanoimprint lithography using a template fabricated by helium ion beam lithography Wen-Di Li*, Wei Wu** and R. Stanley Williams Hewlett-Packard Labs *Current address: University
Ion Beam Sputtering: Practical Applications to Electron Microscopy Applications Laboratory Report Introduction Electron microscope specimens, both scanning (SEM) and transmission (TEM), often require a
Surface plasmon nanophotonics: optics below the diffraction limit Albert Polman Center for nanophotonics FOM-Institute AMOLF, Amsterdam Jeroen Kalkman Hans Mertens Joan Penninkhof Rene de Waele Teun van
Photolithography Figure 12.1. Various ways in which dust particles can interfere with photomask patterns. 19/11/2003 Ettore Vittone- Fisica dei Semiconduttori - Lectio XIII 16 Figure 12.2. Particle-size
Chemical Synthesis Spontaneous organization of molecules into stable, structurally well-defined aggregates at the nanometer length scale. Overview The 1-100 nm nanoscale length is in between traditional
Quantum control of individual electron and nuclear spins in diamond lattice Mikhail Lukin Physics Department, Harvard University Collaborators: L.Childress, M.Gurudev Dutt, J.Taylor, D.Chang, L.Jiang,A.Zibrov
Dry Etching and Reactive Ion Etching (RIE) MEMS 5611 Feb 19 th 2013 Shengkui Gao Contents refer slides from UC Berkeley, Georgia Tech., KU, etc. (see reference) 1 Contents Etching and its terminologies
Kasetsart J. (Nat. Sci.) 42 : 357-361 (28) Phase Characterization of TiO 2 Powder by XRD and TEM Kheamrutai Thamaphat 1 *, Pichet Limsuwan 1 and Boonlaer Ngotawornchai 2 ABSTRACT In this study, the commercial
Satisloh Italy S.r.l. Coating Technology: Evaporation Vs Sputtering Gianni Monaco, PhD R&D project manager, Satisloh Italy 04.04.2016 V1 The aim of this document is to provide basic technical information
www.sciencemag.org/cgi/content/full/1162193/dc1 Supporting Online Material for Polymer Pen Lithography Fengwei Huo, Zijian Zheng, Gengfeng Zheng, Louise R. Giam, Hua Zhang, Chad A. Mirkin* *To whom correspondence
Adviser: dr. Maja Remškar Institut Jožef Stefan January 2010 1 2 3 4 5 6 Fluorescence Raman and surface enhanced Raman 7 Conventional optical microscopy-limited resolution Two broad classes of techniques
Acoustics 8 Paris Plate waves in phononic crystals slabs J.-J. Chen and B. Bonello CNRS and Paris VI University, INSP - 14 rue de Lourmel, 7515 Paris, France firstname.lastname@example.org 41 Acoustics 8 Paris We
Supporting Information Simple and Rapid Synthesis of Ultrathin Gold Nanowires, Their Self-Assembly and Application in Surface-Enhanced Raman Scattering Huajun Feng, a Yanmei Yang, a Yumeng You, b Gongping
Module 7 Wet and Dry Etching Class Notes 1. Introduction Etching techniques are commonly used in the fabrication processes of semiconductor devices to remove selected layers for the purposes of pattern
MMIC Design and Technology Fabrication of MMIC Instructor Dr. Ali Medi Substrate Process Choice Mobility & Peak Velocity: Frequency Response Band-Gap Energy: Breakdown Voltage (Power-Handling) Resistivity:
APPLICATION OF X-RAY COMPUTED TOMOGRAPHY IN SILICON SOLAR CELLS V.A. Popovich 1, W. Verwaal 2, M. Janssen 1, I. J. Bennett 3, I.M.Richardson 1, 1. Delft University of Technology, Department of Materials
1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 Single Defect Center Scanning Near-Field Optical Microscopy on Graphene J. Tisler, T. Oeckinghaus, R. Stöhr, R. Kolesov, F. Reinhard and J. Wrachtrup 3. Institute
Sputtering (cont.) and Other Plasma Processes Sputtering Summary Create an ionic plasma by applying a high voltage to a glow tube. Ions bombard the target material at the cathode. Target atoms are ejected
Solar Photovoltaic (PV) Cells A supplement topic to: Mi ti l S Micro-optical Sensors - A MEMS for electric power generation Science of Silicon PV Cells Scientific base for solar PV electric power generation
JePPIX Course Processing Wet and dry etching processes Huub Ambrosius Material removal: etching processes Etching is done either in dry or wet methods: Wet etching uses liquid etchants with wafers immersed
CONCEPT OF DETERMINISTIC ION IMPLANTATION AT THE NANOSCALE Daniel Spemann Jan Meijer 1, Jürgen W. Gerlach, Paul Räcke 1, Susann Liedtke, Stephan Rauschenbach 2, Bernd Rauschenbach 1 University of Leipzig,
Light Trapping in Silicon Nanowire Solar Cells Erik Garnett and Peidong Yang* Department of Chemistry, University of California, Berkeley, California 94720 pubs.acs.org/nanolett ABSTRACT Thin-film structures
Etching Etch Definitions Isotropic Etching: same in all direction Anisotropic Etching: direction sensitive Selectivity: etch rate difference between 2 materials Other layers below one being etch Masking
International Journal of Arts and Sciences 3(1): 18-26 (2009) CD-ROM. ISSN: 1944-6934 InternationalJournal.org Usage of Carbon Nanotubes in Scanning Probe Microscopes as Probe Bedri Onur Kucukyildirim,
Photolithography Process by which patterns are formed on the surface of the wafer Needed for selective doping and formation of metal interconnects 3 main components Photoresist - light sensitive polymer
berlin Nanoscale Resolution Options for Optical Localization Techniques C. Boit TU Berlin Chair of Semiconductor Devices EUFANET Workshop on Optical Localization Techniques Toulouse, Jan 26, 2009 Jan 26,
Date: Oct. 2007 STS Advanced Silicon Etch DRIE HRM System Trends A- INTRODUCTION The purpose of this document is to help for process development of the ASE DRIE. This document provides general trends but
Lecture 11 Etching Techniques Reading: Chapter 11 Etching Techniques Characterized by: 1.) Etch rate (A/minute) 2.) Selectivity: S=etch rate material 1 / etch rate material 2 is said to have a selectivity
Nano-optical Imaging using Scattering Scanning Near-field Optical Microscopy Fehmi Yasin, Advisor: Dr. Markus Raschke, Post-doc: Dr. Gregory Andreev, Graduate Student: Benjamin Pollard Department of Physics,
Spatially separated excitons in 2D and 1D David Abergel March 10th, 2015 D.S.L. Abergel 3/10/15 1 / 24 Outline 1 Introduction 2 Spatially separated excitons in 2D The role of disorder 3 Spatially separated
Electron Beam and Sputter Deposition Choosing Process Parameters General Introduction The choice of process parameters for any process is determined not only by the physics and/or chemistry of the process,
Integrated Ferroelectrics, 53: 503 511, 2003 Copyright C Taylor & Francis Inc. ISSN: 1058-4587 print/ 1607-8489 online DOI: 10.1080/10584580390258651 Observation of Long Transients in the Electrical Characterization
Subtractive 3D Printing of Optically Active Diamond Structures Aiden A. Martin, Milos Toth *, and Igor Aharonovich School of Physics and Advanced Materials, University of Technology, Sydney, P.O. Box 123,
Structural and optical characterisation of planar waveguides obtained via Sol-Gel F. Rey-García, C. Gómez-Reino, M.T. Flores-Arias, G.F. De La Fuente, W. Assenmacher, W. Mader ABSTRACT Planar waveguides
Sputtering Vacuum Evaporation Recap Use high temperatures at high vacuum to evaporate (eject) atoms or molecules off a material surface. Use ballistic flow to transport them to a substrate and deposit.
Epitaxy Epitaxial Growth Epitaxy means the growth of a single crystal film on top of a crystalline substrate. For most thin film applications (hard and soft coatings, optical coatings, protective coatings)
Electron Microscopy 3. SEM Image formation, detection, resolution, signal to noise ratio, interaction volume, contrasts 3-1 SEM is easy! Just focus and shoot "Photo"!!! Please comment this picture... Any
Modification of Graphene Films by Laser-Generated High Energy Particles Elena Stolyarova (Polyakova), Ph.D. ATF Program Advisory and ATF Users Meeting April 2-3, 2009, Berkner Hall, Room B, BNL Department
TRANSACTIONS ON ELECTRICAL AND ELECTRONIC MATERIALS Vol. 16, No. 2, pp. 90-94, April 25, 2015 Regular Paper pissn: 1229-7607 eissn: 2092-7592 DOI: http://dx.doi.org/10.4313/teem.2015.16.2.90 OAK Central:
Chemical Sputtering von Kohlenstoff durch Wasserstoff W. Jacob Centre for Interdisciplinary Plasma Science Max-Planck-Institut für Plasmaphysik, 85748 Garching Content: Definitions: Chemical erosion, physical
Applied Surface Science 186 2002) 453±457 Exploring the deposition of oxides on silicon for photovoltaic cells by pulsed laser deposition Lianne M. Doeswijk a,*, Hugo H.C. de Moor b, Horst Rogalla a, Dave
Hello and Welcome to this presentation on LED Basics. In this presentation we will look at a few topics in semiconductor lighting such as light generation from a semiconductor material, LED chip technology,
DOE Solar Energy Technologies Program Peer Review Evaluation of Nanocrystalline Silicon Thin Film by Near-Field Scanning Optical Microscopy AAT-2-31605-05 Magnus Wagener and George Rozgonyi North Carolina
QUANTUM DOTS Technology White Papers nr. 13 Paul Holister Cristina Román Vas Tim Harper QUANTUM DOTS Technology White Papers nr. 13 Release Date: Published by Científica Científica, Ltd. www.cientifica.com
Raman spectroscopy Lecture Licentiate course in measurement science and technology Spring 2008 10.04.2008 Antti Kivioja Contents - Introduction - What is Raman spectroscopy? - The theory of Raman spectroscopy
Microsyst Technol (2009) 15:1045 1049 DOI 10.1007/s00542-009-0880-8 TECHNICAL PAPER Femtosecond laser-induced silicon surface morphology in water confinement Yukun Han Æ Cheng-Hsiang Lin Æ Hai Xiao Æ Hai-Lung
Phonon Scattering and Thermal Conduction in Nanostructured Semiconductors David G. Cahill, Joe Feser, Yee Kan Koh Department of Materials Science and Engineering And Materials Research Laboratory University
2 Absorbing Solar Energy 2.1 Air Mass and the Solar Spectrum Now that we have introduced the solar cell, it is time to introduce the source of the energy the sun. The sun has many properties that could
Improved Contact Formation for Large Area Solar Cells Using the Alternative Seed Layer (ASL) Process Lynne Michaelson, Krystal Munoz, Jonathan C. Wang, Y.A. Xi*, Tom Tyson, Anthony Gallegos Technic Inc.,
Graduate Student Presentations Dang, Huong Chip packaging March 27 Call, Nathan Thin film transistors/ liquid crystal displays April 4 Feldman, Ari Optical computing April 11 Guerassio, Ian Self-assembly
contamination analysis for compound semiconductors ANALYTICAL SERVICES B u r i e d d e f e c t s, E v a n s A n a l y t i c a l g r o u p h e l p s y o u C O N T R O L C O N T A M I N A T I O N Contamination
Ultrahigh-efficiency solar cells based on nanophotonic design Albert Polman Piero Spinelli Jorik van de Groep Claire van Lare Bonna Newman Erik Garnett Marc Verschuuren Ruud Schropp Wim Sinke Center for
UNCLASSIFIED Defense Technical Information Center Compilation Part Notice ADP012914 TITLE: Atomic Force Microscopy Characterization of Nanostructured Materials Using Selective Chemical Etching DISTRIBUTION:
Nanoelectronics 09 Atsufumi Hirohata Department of Electronics 12:00 Wednesday, 4/February/2015 (P/L 006) Quick Review over the Last Lecture ( Field effect transistor (FET) ): ( Drain ) current increases
Lecture 12 Physical Vapor Deposition: Evaporation and Sputtering Reading: Chapter 12 Evaporation and Sputtering (Metalization) Evaporation For all devices, there is a need to go from semiconductor to metal.
Vol. 93 (1997) A CTA PHYSICA POLONICA A No. 2 Proceedings of the 1st International Symposium on Scanning Probe Spectroscopy and Related Methods, Poznań 1997 NEAR FIELD OPTICAL MICROSCOPY AND SPECTROSCOPY
Darrick Chang ICFO The Institute of Photonic Sciences Barcelona, Spain April 2, 2014 ICFO The Institute of Photonic Sciences 10 minute walk 11 years old 22 Research Groups 300 people Research themes: Quantum
F. G. Tseng Lec6, Fall/2001, p1 Lecture 6 PVD (Physical vapor deposition): Evaporation and Sputtering Vacuum evaporation 1. Fundamental of Evaporation: The material to be evaporated is heated in an evacuated
Module 3 : Fabrication Process and Layout Design Rules Lecture 12 : CMOS Fabrication Technologies Objectives In this course you will learn the following Introduction Twin Well/Tub Technology Silicon on
The study of deep-level emission center in ZnO films grown on c-al 2 O 3 substrates Guotong Du Yuantao Zhang, Jinzhong Wang, Yongguo Cui (College of Electronic Science and Engineering, State Key Laboratory
Progress In Electromagnetics Research Symposium 2005, Hangzhou, China, August 22-26 331 Broadband THz Generation from Photoconductive Antenna Qing Chang 1, Dongxiao Yang 1,2, and Liang Wang 1 1 Zhejiang
Optical Properties of Sputtered Tantalum Nitride Films Determined by Spectroscopic Ellipsometry Thomas Waechtler a, Bernd Gruska b, Sven Zimmermann a, Stefan E. Schulz a, Thomas Gessner a a Chemnitz University
Spectroscopic : What it is, what it will do, and what it won t do by Harland G. Tompkins Introduction Fundamentals Anatomy of an ellipsometric spectrum Analysis of an ellipsometric spectrum What you can
Thermal unobtainiums? The perfect thermal conductor and the perfect thermal insulator David G. Cahill Materials Research Lab and Department of Materials Science and Engineering, U. of Illinois Gratefully
Silicon-On-Glass MEMS Design Handbook A Process Module for a Multi-User Service Program A Michigan Nanofabrication Facility process at the University of Michigan March 2007 TABLE OF CONTENTS Chapter 1...
Connectivity in a Wireless World Cables Connectors 204 A Special Supplement to Signal Launch Methods for RF/Microwave PCBs John Coonrod Rogers Corp., Chandler, AZ COAX CABLE MICROSTRIP TRANSMISSION LINE
GREEN NANOTECHNOLOGY Solutions for Sustainability and Energy in the Built Environment Geoffrey B. Smith Claes G. Granqvist CRC Press Taylor & Francis Group Boca Raton London NewYork CRC Press is an imprint
First Electrically Pumped Hybrid Silicon Laser Sept 18 th 2006 The information in this presentation is under embargo until 9/18/06 10:00 AM PST 1 Agenda Dr. Mario Paniccia Director, Photonics Technology
Pulsed laser deposition of organic materials PhD theses Gabriella Kecskeméti Department of Optics and Quantum Electronics University of Szeged Supervisor: Dr. Béla Hopp senior research fellow Department
THE USE OF OZONATED HF SOLUTIONS FOR POLYSILICON STRIPPING Gim S. Chen, Ismail Kashkoush, and Rich E. Novak AKrion LLC 633 Hedgewood Drive, #15 Allentown, PA 1816, USA ABSTRACT Ozone-based HF chemistry
Hard Condensed Matter WZI Tom Gregorkiewicz University of Amsterdam VU-LaserLab Dec 10, 2015 Hard Condensed Matter Cluster Quantum Matter Optoelectronic Materials Quantum Matter Amsterdam Mark Golden Anne
Porous silicon based optical multilayers PhD thesis János Volk Supervisor: Dr. István Bársony MTA Research Institute for Technical Physics and Materials Sciences Budapest 2005 Premises Due to the discovery
Properties of optical thin films produced by reactive low voltage ion plating (RLVIP) Antje Hallbauer Thin Film Technology Institute of Ion Physics & Applied Physics University of Innsbruck Investigations
Forensic Science: The Basics Microscopy Chapter 6 Jay A. Siegel,Ph.D. Power point presentation by Greg Galardi, Peru State College, Peru Nebraska Presentation by Greg Galardi, Peru State College CRC Press,